#------------------------------------------------------------------------------
#$Date: 2021-04-05 00:54:45 +0300 (Mon, 05 Apr 2021) $
#$Revision: 263607 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/70/70/7707057.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7707057
loop_
_publ_author_name
'Zhang, Le'
'Liu, Xinxin'
'Shang, Mingyu'
'Sun, Fuxing'
'Jian, Juan'
'Bu, Ke'
'Zeng, Decheng'
'Yuan, Hongming'
_publ_section_title
;
 Efficient proton conductivity of a novel 3D open-framework vanadoborate
 with [V₆B₂₀] architectures.
;
_journal_issue                   9
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              3240
_journal_page_last               3246
_journal_paper_doi               10.1039/d0dt04426a
_journal_volume                  50
_journal_year                    2021
_chemical_formula_sum            'B40 H0 N2 Na6 Ni2 O127.52 V12'
_chemical_formula_weight         3367.38
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2021-02-01 deposited with the CCDC.	2021-02-12 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 117.47(3)
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   12.069(2)
_cell_length_b                   21.876(4)
_cell_length_c                   12.218(2)
_cell_measurement_reflns_used    92174
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.782
_cell_measurement_theta_min      2.645
_cell_volume                     2862.1(12)
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 100cm
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1075
_diffrn_reflns_av_unetI/netI     0.0408
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            92174
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.782
_diffrn_reflns_theta_min         2.645
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    1.422
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    1.954
_exptl_crystal_description       plate
_exptl_crystal_F_000             1632
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.22
_refine_diff_density_max         1.950
_refine_diff_density_min         -1.170
_refine_diff_density_rms         0.175
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.142
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     430
_refine_ls_number_reflns         6099
_refine_ls_number_restraints     6
_refine_ls_restrained_S_all      1.142
_refine_ls_R_factor_all          0.0951
_refine_ls_R_factor_gt           0.0798
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0552P)²+40.0629P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1766
_refine_ls_wR_factor_ref         0.1839
_reflns_Friedel_coverage         0.000
_reflns_number_gt                5167
_reflns_number_total             6099
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d0dt04426a2.cif
_cod_data_source_block           m2
_cod_original_cell_volume        2862.0(12)
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               7707057
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ni1 Ni 1.000000 0.500000 1.000000 0.0077(2) Uani 1 2 d S . P . .
V1 V 0.24605(9) 0.45721(5) 0.80125(9) 0.0069(2) Uani 1 1 d . . . . .
V2 V 0.34675(9) 0.58181(5) 0.77482(9) 0.0077(2) Uani 1 1 d . . . . .
V3 V 0.60113(9) 0.62444(5) 0.97329(9) 0.0072(2) Uani 1 1 d . . . . .
O1 O 0.6887(4) 0.40538(19) 0.9694(4) 0.0078(8) Uani 1 1 d . . . . .
O2 O 0.5041(4) 0.4233(2) 0.7791(4) 0.0097(9) Uani 1 1 d . . . . .
O3 O 0.6636(4) 0.49836(19) 0.8576(4) 0.0070(8) Uani 1 1 d . . . . .
O4 O 0.7012(4) 0.4050(2) 0.7766(4) 0.0134(9) Uani 1 1 d . . . . .
O5 O 0.5366(4) 0.32585(19) 0.8799(4) 0.0102(9) Uani 1 1 d . . . . .
O6 O 0.5768(4) 0.36821(19) 1.0766(4) 0.0099(9) Uani 1 1 d . . . . .
O7 O 0.7273(4) 0.30394(19) 1.0573(4) 0.0107(9) Uani 1 1 d . . . . .
O8 O 0.8580(4) 0.47663(19) 1.0363(4) 0.0074(8) Uani 1 1 d . . . . .
O9 O 0.7651(4) 0.45509(19) 1.1663(4) 0.0088(8) Uani 1 1 d . . . . .
O10 O 0.8909(4) 0.37932(19) 1.1333(4) 0.0090(8) Uani 1 1 d . . . . .
O11 O 0.7361(4) 0.56426(19) 1.0346(4) 0.0090(8) Uani 1 1 d . . . . .
O12 O 0.8493(4) 0.55895(19) 0.9145(4) 0.0081(8) Uani 1 1 d . . . . .
O13 O 0.6660(4) 0.5795(2) 0.7250(4) 0.0106(9) Uani 1 1 d . . . . .
O14 O 0.4936(4) 0.51086(19) 0.6543(4) 0.0099(9) Uani 1 1 d . . . . .
O15 O 0.5237(4) 0.58402(19) 0.8129(4) 0.0086(8) Uani 1 1 d . . . . .
O16 O 0.3432(4) 0.4319(2) 0.5681(4) 0.0119(9) Uani 1 1 d . . . . .
O17 O 0.3383(4) 0.49684(19) 0.7243(4) 0.0084(8) Uani 1 1 d . . . . .
O18 O 0.3645(4) 0.3388(2) 0.6813(4) 0.0110(9) Uani 1 1 d . . . . .
O19 O 0.3634(4) 0.38842(19) 0.8549(4) 0.0095(9) Uani 1 1 d . . . . .
O20 O 0.9405(4) 0.2767(2) 1.1794(5) 0.0196(11) Uani 1 1 d . . . . .
O21 O 0.8624(4) 0.6080(2) 0.7482(4) 0.0203(11) Uani 1 1 d . . . . .
O22 O 0.2450(6) 0.3397(2) 0.4678(5) 0.0268(12) Uani 1 1 d . . . . .
O23 O 0.1143(4) 0.4332(2) 0.6966(4) 0.0153(10) Uani 1 1 d . . . . .
O24 O 0.2645(4) 0.6245(2) 0.6571(4) 0.0177(10) Uani 1 1 d . . . . .
O25 O 0.6564(4) 0.6897(2) 0.9610(5) 0.0166(10) Uani 1 1 d . . . . .
O26 O 0.9306(4) 0.4458(2) 0.8437(4) 0.0167(10) Uani 1 1 d . . . . .
B1 B 0.6401(6) 0.4313(3) 0.8443(6) 0.0090(13) Uani 1 1 d . U . . .
B2 B 0.6281(6) 0.3493(3) 0.9945(6) 0.0084(13) Uani 1 1 d . . . . .
B3 B 0.8045(6) 0.4299(3) 1.0798(6) 0.0069(12) Uani 1 1 d . . . . .
B4 B 0.7759(6) 0.5251(3) 0.9650(6) 0.0084(13) Uani 1 1 d . . . . .
B5 B 0.5816(6) 0.5444(3) 0.7574(6) 0.0092(13) Uani 1 1 d . . . . .
B6 B 0.4185(6) 0.4681(3) 0.6784(6) 0.0097(13) Uani 1 1 d . . . . .
B7 B 0.4420(7) 0.3668(3) 0.8026(7) 0.0103(13) Uani 1 1 d . . . . .
B8 B 0.8496(7) 0.3198(3) 1.1211(7) 0.0104(13) Uani 1 1 d . . . . .
B9 B 0.7921(7) 0.5825(3) 0.7970(7) 0.0111(13) Uani 1 1 d . . . . .
B10 B 0.3194(7) 0.3713(4) 0.5749(7) 0.0127(14) Uani 1 1 d . . . . .
Na1 Na 0.6137(4) 0.2342(2) 0.8669(4) 0.0281(9) Uiso 0.75 1 d . . P A 1
Na2 Na 0.5815(12) 0.2251(6) 0.9128(12) 0.029(3) Uiso 0.25 1 d . . P A 2
O27 O 0.7383(8) 0.2775(4) 0.7795(8) 0.042(2) Uiso 0.75 1 d . . P . .
O28A O 0.4573(15) 0.2021(8) 0.9620(15) 0.057(4) Uiso 0.5 1 d . . P A 1
O28B O 0.495(2) 0.1677(13) 0.952(2) 0.038(6) Uiso 0.25 1 d . . P A 2
Na3 Na 0.5898(7) 0.4515(4) 0.5533(7) 0.0425(18) Uiso 0.5 1 d . . P . .
O29A O 0.8054(12) 0.4685(6) 0.5768(11) 0.032(3) Uiso 0.5 1 d . . P B 1
O29B O 0.855(3) 0.4844(13) 0.571(2) 0.039(6) Uiso 0.25 1 d . . P C 2
O30A O 0.574(3) 0.3758(13) 0.515(3) 0.063(7) Uiso 0.33 1 d . . P B 1
O32A O 0.4528(17) 0.3025(9) 0.3439(17) 0.035(4) Uiso 0.33 1 d . . P D 1
O30B O 0.5218(18) 0.3496(9) 0.4614(17) 0.033(4) Uiso 0.33 1 d . . P B 2
O31A O 0.6692(16) 0.2808(7) 0.5284(15) 0.022(3) Uiso 0.33 1 d . . P E 2
O31B O 0.611(3) 0.2698(12) 0.530(2) 0.062(7) Uiso 0.33 1 d . . P F 3
O32B O 0.515(2) 0.2758(11) 0.318(2) 0.052(6) Uiso 0.33 1 d . . P G 3
O33 O 0.0637(11) 0.3311(5) 0.8781(11) 0.051(3) Uiso 0.65 1 d . . P . .
O34A O 0.187(3) 0.2644(15) 0.750(3) 0.054(8) Uiso 0.25 1 d . . P H 1
O34B O 0.1426(10) 0.2838(5) 0.6945(10) 0.054(3) Uiso 0.75 1 d . . P I 2
N1 N -0.004(2) 0.4417(10) 0.426(2) 0.064(5) Uiso 0.5 1 d . . P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O8 Ni1 O8 180.0(2) . 3_767 ?
O8 Ni1 O26 88.02(18) . 3_767 ?
O8 Ni1 O26 91.98(18) 3_767 3_767 ?
O8 Ni1 O26 91.98(18) . . ?
O8 Ni1 O26 88.02(18) 3_767 . ?
O26 Ni1 O26 180.0 3_767 . ?
O8 Ni1 O12 68.49(16) . . ?
O8 Ni1 O12 111.51(16) 3_767 . ?
O26 Ni1 O12 89.76(18) 3_767 . ?
O26 Ni1 O12 90.24(18) . . ?
O8 Ni1 O12 111.51(16) . 3_767 ?
O8 Ni1 O12 68.49(16) 3_767 3_767 ?
O26 Ni1 O12 90.24(18) 3_767 3_767 ?
O26 Ni1 O12 89.76(18) . 3_767 ?
O12 Ni1 O12 180.0(3) . 3_767 ?
O23 V1 O17 109.7(2) . . ?
O23 V1 O19 108.3(2) . . ?
O17 V1 O19 91.00(18) . . ?
O23 V1 O11 109.6(2) . 3_667 ?
O17 V1 O11 140.66(18) . 3_667 ?
O19 V1 O11 75.77(18) . 3_667 ?
O23 V1 O9 110.1(2) . 3_667 ?
O17 V1 O9 76.85(17) . 3_667 ?
O19 V1 O9 141.59(19) . 3_667 ?
O11 V1 O9 90.75(18) 3_667 3_667 ?
O23 V1 V2 120.27(17) . . ?
O17 V1 V2 38.22(12) . . ?
O19 V1 V2 117.26(13) . . ?
O11 V1 V2 117.18(13) 3_667 . ?
O9 V1 V2 39.07(12) 3_667 . ?
O23 V1 V3 119.23(18) . 3_667 ?
O17 V1 V3 116.56(13) . 3_667 ?
O19 V1 V3 38.18(13) . 3_667 ?
O11 V1 V3 38.13(12) 3_667 3_667 ?
O9 V1 V3 116.85(13) 3_667 3_667 ?
V2 V1 V3 120.49(5) . 3_667 ?
O24 V2 O17 110.4(2) . . ?
O24 V2 O6 109.7(2) . 3_667 ?
O17 V2 O6 139.85(18) . 3_667 ?
O24 V2 O15 110.5(2) . . ?
O17 V2 O15 89.48(18) . . ?
O6 V2 O15 76.70(18) 3_667 . ?
O24 V2 O9 108.6(2) . 3_667 ?
O17 V2 O9 77.27(17) . 3_667 ?
O6 V2 O9 89.98(18) 3_667 3_667 ?
O15 V2 O9 140.88(18) . 3_667 ?
O24 V2 V3 120.71(19) . . ?
O17 V2 V3 115.49(13) . . ?
O6 V2 V3 38.51(13) 3_667 . ?
O15 V2 V3 38.67(13) . . ?
O9 V2 V3 116.26(13) 3_667 . ?
O24 V2 V1 119.87(19) . . ?
O17 V2 V1 38.53(12) . . ?
O6 V2 V1 116.22(13) 3_667 . ?
O15 V2 V1 115.97(13) . . ?
O9 V2 V1 39.19(12) 3_667 . ?
V3 V2 V1 119.42(4) . . ?
O25 V3 O6 109.9(2) . 3_667 ?
O25 V3 O15 109.5(2) . . ?
O6 V3 O15 77.00(18) 3_667 . ?
O25 V3 O11 109.0(2) . . ?
O6 V3 O11 141.11(19) 3_667 . ?
O15 V3 O11 90.48(18) . . ?
O25 V3 O19 109.4(2) . 3_667 ?
O6 V3 O19 90.68(18) 3_667 3_667 ?
O15 V3 O19 141.06(18) . 3_667 ?
O11 V3 O19 76.17(18) . 3_667 ?
O25 V3 V2 120.29(18) . . ?
O6 V3 V2 38.48(13) 3_667 . ?
O15 V3 V2 39.00(13) . . ?
O11 V3 V2 117.00(13) . . ?
O19 V3 V2 116.75(14) 3_667 . ?
O25 V3 V1 119.62(18) . 3_667 ?
O6 V3 V1 116.50(13) 3_667 3_667 ?
O15 V3 V1 116.57(13) . 3_667 ?
O11 V3 V1 38.53(13) . 3_667 ?
O19 V3 V1 38.19(13) 3_667 3_667 ?
V2 V3 V1 120.09(5) . 3_667 ?
B1 O1 B3 123.1(5) . . ?
B1 O1 B2 121.2(5) . . ?
B3 O1 B2 115.7(4) . . ?
B1 O2 B7 121.0(5) . . ?
B1 O2 B6 121.8(5) . . ?
B7 O2 B6 117.1(5) . . ?
B1 O3 B4 122.0(5) . . ?
B1 O3 B5 122.5(5) . . ?
B4 O3 B5 115.4(5) . . ?
B1 O4 Na3 106.6(4) . . ?
B7 O5 B2 116.7(5) . . ?
B7 O5 Na1 138.7(4) . . ?
B2 O5 Na1 103.5(4) . . ?
B7 O5 Na2 142.1(5) . . ?
B2 O5 Na2 99.4(5) . . ?
B2 O6 V2 129.1(4) . 3_667 ?
B2 O6 V3 124.3(4) . 3_667 ?
V2 O6 V3 103.0(2) 3_667 3_667 ?
B8 O7 B2 122.4(5) . . ?
B8 O7 Na2 143.3(5) . . ?
B2 O7 Na2 87.6(5) . . ?
B8 O7 Na1 130.7(4) . . ?
B2 O7 Na1 87.8(4) . . ?
B3 O8 B4 116.6(5) . . ?
B3 O8 Ni1 146.3(4) . . ?
B4 O8 Ni1 95.6(3) . . ?
B3 O9 V2 128.2(4) . 3_667 ?
B3 O9 V1 126.1(4) . 3_667 ?
V2 O9 V1 101.73(19) 3_667 3_667 ?
B8 O10 B3 121.5(5) . . ?
B4 O11 V3 128.4(4) . . ?
B4 O11 V1 123.4(4) . 3_667 ?
V3 O11 V1 103.3(2) . 3_667 ?
B9 O12 B4 120.7(5) . . ?
B9 O12 Ni1 131.3(4) . . ?
B4 O12 Ni1 91.9(3) . . ?
B9 O13 B5 123.9(5) . . ?
B5 O14 B6 116.2(5) . . ?
B5 O14 Na3 122.5(4) . 3_666 ?
B6 O14 Na3 116.6(4) . 3_666 ?
B5 O14 Na3 113.0(4) . . ?
B6 O14 Na3 104.7(4) . . ?
Na3 O14 Na3 73.3(3) 3_666 . ?
B5 O15 V3 128.6(4) . . ?
B5 O15 V2 125.1(4) . . ?
V3 O15 V2 102.33(19) . . ?
B10 O16 B6 121.9(5) . . ?
B6 O17 V2 125.7(4) . . ?
B6 O17 V1 128.0(4) . . ?
V2 O17 V1 103.24(19) . . ?
B10 O18 B7 122.3(5) . . ?
B7 O19 V3 124.2(4) . 3_667 ?
B7 O19 V1 128.6(4) . . ?
V3 O19 V1 103.6(2) 3_667 . ?
B8 O20 Na1 137.1(5) . 4_666 ?
B8 O20 Na2 123.4(5) . 4_666 ?
Na1 O20 Na2 18.9(3) 4_666 4_666 ?
B10 O22 Na1 152.0(5) . 4_565 ?
B10 O22 Na2 133.7(6) . 4_565 ?
Na1 O22 Na2 21.6(3) 4_565 4_565 ?
O4 B1 O2 112.1(5) . . ?
O4 B1 O1 111.8(5) . . ?
O2 B1 O1 109.1(5) . . ?
O4 B1 O3 109.3(5) . . ?
O2 B1 O3 106.7(5) . . ?
O1 B1 O3 107.5(5) . . ?
O5 B2 O6 113.4(5) . . ?
O5 B2 O7 110.3(5) . . ?
O6 B2 O7 109.5(5) . . ?
O5 B2 O1 108.6(5) . . ?
O6 B2 O1 107.7(5) . . ?
O7 B2 O1 107.2(5) . . ?
O5 B2 Na2 51.2(4) . . ?
O6 B2 Na2 115.6(5) . . ?
O7 B2 Na2 61.5(4) . . ?
O1 B2 Na2 136.6(5) . . ?
O5 B2 Na1 48.3(3) . . ?
O6 B2 Na1 132.1(4) . . ?
O7 B2 Na1 62.0(3) . . ?
O1 B2 Na1 120.0(4) . . ?
O8 B3 O10 110.9(5) . . ?
O8 B3 O9 110.7(5) . . ?
O10 B3 O9 111.7(5) . . ?
O8 B3 O1 108.0(5) . . ?
O10 B3 O1 107.8(5) . . ?
O9 B3 O1 107.7(5) . . ?
O11 B4 O8 113.9(5) . . ?
O11 B4 O12 112.0(5) . . ?
O8 B4 O12 104.0(5) . . ?
O11 B4 O3 109.6(5) . . ?
O8 B4 O3 109.4(5) . . ?
O12 B4 O3 107.6(5) . . ?
O14 B5 O15 113.3(5) . . ?
O14 B5 O13 111.0(5) . . ?
O15 B5 O13 110.8(5) . . ?
O14 B5 O3 108.1(5) . . ?
O15 B5 O3 106.8(5) . . ?
O13 B5 O3 106.5(5) . . ?
O14 B6 O16 110.4(5) . . ?
O14 B6 O17 113.2(5) . . ?
O16 B6 O17 110.2(5) . . ?
O14 B6 O2 109.1(5) . . ?
O16 B6 O2 107.1(5) . . ?
O17 B6 O2 106.6(5) . . ?
O14 B6 Na3 49.0(3) . . ?
O16 B6 Na3 75.8(4) . . ?
O17 B6 Na3 160.9(5) . . ?
O2 B6 Na3 88.0(4) . . ?
O5 B7 O19 113.8(5) . . ?
O5 B7 O18 110.5(5) . . ?
O19 B7 O18 109.8(5) . . ?
O5 B7 O2 108.7(5) . . ?
O19 B7 O2 107.2(5) . . ?
O18 B7 O2 106.5(5) . . ?
O7 B8 O20 121.3(6) . . ?
O7 B8 O10 123.1(6) . . ?
O20 B8 O10 115.5(6) . . ?
O21 B9 O13 118.2(6) . . ?
O21 B9 O12 119.8(6) . . ?
O13 B9 O12 122.0(6) . . ?
O18 B10 O16 124.3(6) . . ?
O18 B10 O22 116.3(6) . . ?
O16 B10 O22 119.4(6) . . ?
O22 Na1 O5 146.2(3) 4_666 . ?
O22 Na1 O20 124.9(3) 4_666 4_565 ?
O5 Na1 O20 87.0(2) . 4_565 ?
O22 Na1 O27 95.8(3) 4_666 . ?
O5 Na1 O27 92.6(3) . . ?
O20 Na1 O27 93.8(3) 4_565 . ?
O22 Na1 O7 89.1(2) 4_666 . ?
O5 Na1 O7 58.31(18) . . ?
O20 Na1 O7 145.3(2) 4_565 . ?
O27 Na1 O7 89.2(3) . . ?
O22 Na1 O28A 91.9(4) 4_666 . ?
O5 Na1 O28A 79.0(4) . . ?
O20 Na1 O28A 84.7(4) 4_565 . ?
O27 Na1 O28A 171.5(5) . . ?
O7 Na1 O28A 87.3(4) . . ?
O22 Na1 B2 118.9(3) 4_666 . ?
O5 Na1 B2 28.17(18) . . ?
O20 Na1 B2 115.2(2) 4_565 . ?
O27 Na1 B2 90.2(3) . . ?
O7 Na1 B2 30.16(16) . . ?
O28A Na1 B2 83.0(4) . . ?
O28B Na2 O5 126.6(11) . . ?
O5 Na2 O22 140.1(7) . 4_666 ?
O28B Na2 O7 125.9(11) . . ?
O5 Na2 O7 59.3(3) . . ?
O22 Na2 O7 89.4(5) 4_666 . ?
O5 Na2 O20 80.5(4) . 4_565 ?
O22 Na2 O20 111.2(6) 4_666 4_565 ?
O7 Na2 O20 133.1(6) . 4_565 ?
O28B Na2 B2 127.2(11) . . ?
O5 Na2 B2 29.3(2) . . ?
O22 Na2 B2 119.2(5) 4_666 . ?
O7 Na2 B2 30.9(2) . . ?
O20 Na2 B2 109.0(5) 4_565 . ?
O30A Na3 O14 96.1(10) . 3_666 ?
O30A Na3 O14 129.7(10) . . ?
O14 Na3 O14 106.7(3) 3_666 . ?
O14 Na3 O30B 86.5(5) 3_666 . ?
O14 Na3 O30B 125.5(6) . . ?
O30A Na3 O29A 99.0(10) . . ?
O14 Na3 O29A 88.7(4) 3_666 . ?
O14 Na3 O29A 125.2(4) . . ?
O30A Na3 O4 81.2(10) . . ?
O14 Na3 O4 173.6(4) 3_666 . ?
O14 Na3 O4 79.3(3) . . ?
O30B Na3 O4 91.5(5) . . ?
O29A Na3 O4 86.1(4) . . ?
O30A Na3 Na3 128.7(11) . 3_666 ?
O14 Na3 Na3 53.7(3) 3_666 3_666 ?
O14 Na3 Na3 53.0(3) . 3_666 ?
O30B Na3 Na3 116.0(6) . 3_666 ?
O29A Na3 Na3 117.8(5) . 3_666 ?
O4 Na3 Na3 132.3(5) . 3_666 ?
O30A Na3 B6 103.3(10) . . ?
O14 Na3 B6 115.4(3) 3_666 . ?
O14 Na3 B6 26.34(18) . . ?
O30B Na3 B6 100.0(5) . . ?
O29A Na3 B6 144.7(4) . . ?
O4 Na3 B6 70.9(2) . . ?
Na3 Na3 B6 66.7(3) 3_666 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ni1 O8 2.024(4) . ?
Ni1 O8 2.024(4) 3_767 ?
Ni1 O26 2.068(5) 3_767 ?
Ni1 O26 2.069(5) . ?
Ni1 O12 2.075(4) . ?
Ni1 O12 2.076(4) 3_767 ?
V1 O23 1.601(5) . ?
V1 O17 1.959(4) . ?
V1 O19 1.960(4) . ?
V1 O11 1.972(4) 3_667 ?
V1 O9 1.976(4) 3_667 ?
V1 V2 3.0616(15) . ?
V1 V3 3.0809(17) 3_667 ?
V2 O24 1.616(5) . ?
V2 O17 1.946(4) . ?
V2 O6 1.948(5) 3_667 ?
V2 O15 1.965(4) . ?
V2 O9 1.971(4) 3_667 ?
V2 V3 3.0506(19) . ?
V3 O25 1.612(5) . ?
V3 O6 1.950(4) 3_667 ?
V3 O15 1.951(4) . ?
V3 O11 1.955(4) . ?
V3 O19 1.960(4) 3_667 ?
O1 B1 1.475(8) . ?
O1 B3 1.523(8) . ?
O1 B2 1.530(8) . ?
O2 B1 1.467(8) . ?
O2 B7 1.539(8) . ?
O2 B6 1.539(8) . ?
O3 B1 1.488(8) . ?
O3 B4 1.503(8) . ?
O3 B5 1.541(8) . ?
O4 B1 1.458(8) . ?
O4 Na3 2.627(9) . ?
O5 B7 1.416(8) . ?
O5 B2 1.420(8) . ?
O5 Na1 2.246(6) . ?
O5 Na2 2.260(14) . ?
O6 B2 1.461(8) . ?
O7 B8 1.358(8) . ?
O7 B2 1.470(8) . ?
O7 Na2 2.514(14) . ?
O7 Na1 2.584(6) . ?
O8 B3 1.436(8) . ?
O8 B4 1.439(8) . ?
O9 B3 1.454(8) . ?
O10 B8 1.378(8) . ?
O10 B3 1.452(8) . ?
O11 B4 1.437(8) . ?
O12 B9 1.374(8) . ?
O12 B4 1.488(8) . ?
O13 B9 1.364(8) . ?
O13 B5 1.469(8) . ?
O14 B5 1.421(8) . ?
O14 B6 1.426(8) . ?
O14 Na3 2.402(9) 3_666 ?
O14 Na3 2.424(9) . ?
O15 B5 1.461(8) . ?
O16 B10 1.367(9) . ?
O16 B6 1.462(8) . ?
O17 B6 1.465(8) . ?
O18 B10 1.357(9) . ?
O18 B7 1.473(8) . ?
O19 B7 1.446(8) . ?
O20 B8 1.371(8) . ?
O20 Na1 2.292(7) 4_666 ?
O20 Na2 2.559(14) 4_666 ?
O21 B9 1.363(8) . ?
O22 B10 1.382(9) . ?
O22 Na1 2.202(7) 4_565 ?
O22 Na2 2.267(14) 4_565 ?
B2 Na2 2.859(15) . ?
B2 Na1 2.924(8) . ?
B6 Na3 3.108(11) . ?
Na1 O27 2.404(10) . ?
Na1 O28A 2.726(17) . ?
Na2 O28B 1.83(3) . ?
Na3 O30A 1.70(3) . ?
Na3 O30B 2.46(2) . ?
Na3 O29A 2.511(16) . ?
Na3 Na3 2.881(16) 3_666 ?
